# Overcapping wax: an aesthetic or functional element

María Ureña, Julie Chanut, Vincent Bottreau, Jean Pierre Bellat, Régis D. Gougeon, Aurélie Lagorce, Thomas Karbowiak

► To cite this version:

María Ureña, Julie Chanut, Vincent Bottreau, Jean Pierre Bellat, Régis D. Gougeon, et al.. Overcapping wax: an aesthetic or functional element. IVES Technical Reviews vine and wine, 2025, pp.1-2. 10.20870/IVES-TR.2025.9182 . hal-04994491

HAL Id: hal-04994491

https://institut-agro-dijon.hal.science/hal-04994491v1

Submitted on 17 Mar 2025

HAL is a multi-disciplinary open access
archive for the deposit and dissemination of sci-
entific research documents, whether they are pub-
lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.

L'archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d'enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.

<figure><img src="image_1.png" /></figure>

Distributed under a Creative Commons Attribution 4.0 International License
<figure><img src="image_2.png" /></figure>

# Overcapping wax: an aesthetic or functional element

María Ureña<fnref n="1" />, Julie Chanut¹³, Vincent Bottreau<fnref n="2" />, Jean-Pierre Bellat<fnref n="3" />, Régis D. Gougeon¹⁴, Aurélie Lagorce<fnref n="1" />, Thomas Karbowiak<fnref n="1" />

An in-depth study was carried out to assess oxygen transfer through different waxes and resins, either alone or used in combination with cork-based stoppers. The research provided the answer to a crucial question being asked by many winemakers and consumers: does the application of overcapping wax play a protective role against oxidation of the wine during bottle ageing?<fnref n="1" />

## Background to the study

The use of waxes and resins in oenology for corking goes back several thousand years, as several archaeological discoveries attest. This empirical use is mainly associated with the idea that they can limit the wine's exposure to oxygen. However, despite this historical use, the exact role of waxes and resins as oxygen barriers has rarely been studied, and even less so as overcapping materials. The only studies into the oxygen permeability of different types of wax (including beeswax, microcrystalline wax and paraffin) were carried out over two decades ago on wax films of relatively thin thickness for applications where wax is used as a food coating<fnref n="2" /> or as a surface treatment agent for cork stoppers<fnref n="3" />. The aim of this study was to evaluate the oxygen barrier properties of different waxes and resins, either alone or in combination with cork-based stoppers. Oxygen transfer through corked bottles, with and without cork wax, was monitored over a one-year storage period.

## Does the sealing wax act as an effective oxygen barrier?

A preliminary step in this study was to characterise the oxygen permeability of various waxes and resins (beeswax, shellac, microcrystalline wax and a commercial blend of waxes), in the form of thin films approximately 350 µm thick. The results show that not all waxes and resins offer an equivalent level of protection (Figure 1). Their effectiveness as oxygen barriers depends mainly on their intrinsic chemical composition and their physical state<fnref n="4" /> ⁵ ⁶.

<figure><img src="image_3.png" /></figure>

**FIGURE 1.** Oxygen barrier properties (in mg.yr⁻<fnref n="1" />) of four waxes and resins, measured at 25°C and 50% relative humidity. The OTR (Oxygen Transmission Rate) values were calculated for a film with a thickness of 350 µm and a diameter of 18.5 mm at an oxygen differential pressure of 212 hPa. The letters in the histogram indicate significant differences between the mean values (p ≤ 0.05, n = 3).

Following this characterisation, the material with the highest oxygen barrier, in this case the wax blend, was selected to evaluate the performance of this wax as an overcapping system on clear glass bottles (37.5 cl capacity). A sensor was placed inside the bottles beforehand to enable the quantity of oxygen entering the bottle to be detected by chemiluminescence. The bottles were used empty to eliminate the influence of the wine and to focus solely on characterising the closure system (bottle + cork +/- wax). Before corking, the bottles were inerted with nitrogen to eliminate the oxygen initially present inside. They were then capped under vacuum using a semi-automatic Bottling machine (GAI 4040WL). The initial partial pressure of oxygen inside the bottles remained below 0.5 hPa. Two types of stoppers were used in the experiments: natural corks, 49 mm long and 24 mm in diameter, and micro-agglomerated corks, 44 mm long and 24 mm in diameter. Some of the corks were also used without surface treatment to simulate a leak at the glass/cork interface. The corks were inserted 3.5 mm below the neck of the bottle to allow sufficient space for subsequent wax deposition. Six replicates were prepared for each condition with micro-agglomerated corks and nine replicates for those with natural corks. Once the bottles had been corked, the wax was deposited, melting it at 120°C before it was deposited on the cork up to the neck of the bottle, which had been heated to 70°C beforehand. The quantity of wax deposited was approximately 1 g, corresponding to a thickness of approximately 3.5 mm once solidified. In the case of surface-treated corks, the wax was applied one month after corking to avoid deformation of the wax disc caused by outgassing of the cork following its compression in the bottleneck. In contrast, for corks without surface treatment (TDS), the wax was added immediately after corking to avoid immediate and excessive oxygen transfer at the glass/cork interface. The samples were stored under controlled conditions at 25°C and 50% relative humidity for the duration of the study. The kinetics of oxygen transfer from the outside to the inside of the bottle were monitored for one year.

The results showed that the use of an overcapping wax leads to different results, depending on the initial oxygen barrier performance of the wax and that of the corks. On one hand, in the case of the micro-agglomerated corks used in this study, the barrier performance of the cork was already found to be very high, being of the same order of magnitude as that of the wax disc (Figure 2a). Consequently, the addition of wax to these stoppers did not confer any additional protection against oxygen (Figure 2b). On the other hand, the greater variability in oxygen permeability of natural cork stoppers (Figure 3a), widely described in the literature⁷ ⁸ ⁹, does not allow the role of wax addition to be accurately assessed (Figure 3b). Finally, in the case of corks without surface treatment (Figure 2c and 3c, "without TDS"), whether natural or micro-agglomerated, very significant oxygen transfer at the glass/cork interface occurs rapidly and is equivalent to a leakage-type defect. In this case, the addition of wax can

<footnote n="1">¹Université Bourgogne Europe, Institut Agro, INRAE, UMR PAM, 21000 Dijon, France</footnote>

<footnote n="2">²Domaine d'Ardhuy, Clos des Langres, 21700 Corgoloin, France</footnote>

<footnote n="3">³Laboratoire Interdisciplinaire Carnot de Bourgogne, UMR 6303 CNRS, 9 Avenue Alain Savary, Dijon 21000, France</footnote>

<footnote n="4">⁴Institut Universitaire de la Vigne et du Vin, 1 rue Claude Ladrey, 21000 Dijon, France</footnote>
<figure><img src="image_4.png" /><figcaption>**FIGURE 2.** Quantity of oxygen entering bottles corked with micro-agglomerated corks (n = 6 for each case studied). (a) Stoppers with surface treatment (TDS) and without the addition of wax. (b) Stoppers with TDS and with the addition of a disk of wax (3.5 mm thick). (c) Stoppers without TDS and without wax. (d) Stoppers without TDS and with the addition of a disk of wax. For waxed conditions, as indicated by the red arrow, the wax was applied 1 month after corking for corks with TDS and the same day for corks without TDS. Mean values and standard deviations are reported for each kinetic.</figcaption></figure>

<figure><img src="image_5.png" /><figcaption>**FIGURE 3.** Quantity of oxygen entering bottles corked with natural cork stoppers (n = 9 for each case studied). (a) Stoppers with surface treatment (TDS) and without the addition of wax. (b) Stoppers with TDS and with the addition of a disk of wax (3.5 mm thick). (c) Stoppers without TDS and without wax. (d) Stoppers without TDS and with the addition of a disk of wax. For waxed conditions, as indicated by the red arrow, the wax was applied 1 month after corking for corks with TDS and the same day for corks without TDS. Due to the variability observed for study cases a and b, the kinetics for each sample are reported individually, whereas for cases c and d, mean values and standard deviations are reported.</figcaption></figure>

considerably limit leakage at the glass/stopper interface (Figure 2d and 3d), thus compensating for the absence of surface treatment¹⁰ ¹¹.

## Conclusions

Waxes and resins have oxygen barrier properties that differ according to their chemical composition. For their application as an overcapping agent, regardless of the type of stopper considered, if the stopper has a lower permeability than the wax and a surface treatment that effectively limits transfer at the glass/stopper interface, the wax will play an aesthetic rather than a functional role.

If we extrapolate the results obtained on corks without surface treatment to the case of defective corks that would lead to high oxygen transfer (high intrinsic permeability and/or inadequate surface treatment), the application of wax would limit excessive oxygen ingress. However, in practice, the wax should not be applied immediately after corking to avoid any deformation of the cork, contrary to what was done in this study for corks without surface treatment. Instead, a period of at least one month should be observed, a critical period during which a significant ingress of oxygen would already have occurred. This study was carried out over a period of one year under laboratory conditions (on empty bottles with constant external temperature and relative humidity). With regard to the longer-term storage of wine in bottles, other questions remain, such as the impact of cork hydration on the oxygen barrier properties of the cork and wax, and the evolution of the physico-chemical properties of the cork and wax over time as a function of storage conditions.

**Acknowledgements:** The authors would like to thank SARL Domaine de la Juvinière (part of Domaine d'Ardhuy) and the Agence Nationale de la Recherche (ANR) as part of the France Relance programme. They would also like to thank the DIVVA platform (Institut Agro Dijon, Université de Bourgogne) for access to analytical equipment, and the Bureau Interprofessionnel des Vins de Bourgogne (BIVB) for the use of an industrial corking machine. Special thanks go to Thomas Chekroun and Éric Néault from Domaine d'Ardhuy for their contribution to the trials.

1. Ureña, M., Chanut, J., Bottreau, V., Bellat, J.-P., Gougeon, R. D., Lagorce, A., & Karbowiak, T. (2024). Wine bottle overcapping wax: An aesthetic or functional element? *Food Packaging and Shelf Life*, 46, 101367. https://doi.org/10.1016/j.fpsl.2024.101367

2. Donhowe, G., & Fennema, O. (1993). Water vapor and oxygen permeability of wax films. *Journal of the American Oil Chemists' Society*, 70(9), 867-873. https://doi.org/10.1007/BF02545345

3. Keenan, C. P., Gözükara, M. Y., Christie, G. B. Y., & Heyes, D. N. (1999). Oxygen permeability of macrocrystalline paraffin wax and relevance to wax coatings on natural corks used as wine bottle closures. *Australian Journal of Grape and Wine Research*, 5(2), 66-70. https://doi.org/10.1111/j.1755-0238.1999.tb00154.x

4. Franke, K., Bindrich, U., & Heinz, V. (2015). Fat crystal network structures have a strong influence on properties of fat-based barrier layers. *European Journal of Lipid Science and Technology*, 117(11), 1792-1800. https://doi.org/10.1002/ejlt.201400576

5. Kester, J. J., & Fennema, O. (1989). The influence of polymorphic form on oxygen and water vapor transmission through lipid films. *Journal of the American Oil Chemists' Society*, 66(8), 1147-1153. https://doi.org/10.1007/BF02670101

6. Martini, S., Kim, D. A., Ollivon, M., & Marangoni, A. G. (2006). Structural factors responsible for the permeability of water vapor through fat barrier films. *Food Research International*, 39(5), 550-558. https://doi.org/10.1016/j.foodres.2005.11.001

7. Chanut, J., Lagorce, A., Lequin, S., Gougeon, R. D., Simon, J.-M., Bellat, J.-P., & Karbowiak, T. (2021a). Fast manometric method for determining the effective oxygen diffusion coefficient through wine stopper. *Polymer Testing*, 93, 106924. https://doi.org/10.1016/j.polymertesting.2020.106924

8. Chevalier, V., Alexandre, P., & Christophe, L. (2019). Impact de l'oubturateur sur le viellissement des vins en bouteille. Partie 1/3—Caractérisation des transferts d'oxygène de bouchons de liège. *Revue des oenologues*, 170, 40-43

9. Oliveira, V., Lopes, P., Cabral, M., & Pereira, H. (2013). Kinetics of Oxygen Ingress into Wine Bottles Closed with Natural Cork Stoppers of Different Qualities. *American Journal of Enology and Viticulture*, 64(3), 395-399. https://doi.org/10.5344/ajev.2013.13009

10. Lagorce-Tachon, A., Karbowiak, T., Paulin, C., Simon, J.-M., Gougeon, R. D., & Bellat, J.-P. (2016). About the Role of the Bottleneck/Cork Interface on Oxygen Transfer. *Journal of Agricultural and Food Chemistry*, 64, 6672-6675. https://doi.org/10.1021/acs.jafc.6b02465

11. Chanut, J., Bellat, J.-P., Gougeon, R. D., & Karbowiak, T. (2021b). Controlled diffusion by thin layer coating: The intricate case of the glass-stopper interface. *Food Control*, 120, 107446. https://doi.org/10.1016/j.foodcont.2020.107446

<figure><img src="image_6.png" /></figure>